August 19, 2014 1
Modeling Tools for SOFC Design and Analysis:Recent PNNL Progress
BRIAN J. KOEPPELK. LAI, W. XU, K. AGARWAL, E.V. STEPHENS, Z. XUPacific Northwest National Laboratory, Richland, WA15th Annual SECA Workshop, Pittsburgh, PA
PNNL Modeling Focus
1. Develop stack modeling toolsSOFC-MP 2D/3D: Multi-physics solver for computing the coupled flow-thermal-electrochemical response of multi-cell SOFC stacksSOFC-ROM: Creation of high fidelity reduced order model (ROM) for use in system-level studiesUser Interface: Make these tools accessible to stack designers
2. Develop models to improve component durability Compliant Seals: Damage-healing constitutive model for study of seal designsInterconnects: Model to evaluate effects of surface modifications and coatings on durability and lifetime
August 19, 2014 2
Summary of Accomplishments
Stack Modeling ToolsCoupled 3D SOFC-MP tool with ANSYS and ABAQUS finite element codes for structural analysisCreated a graphical user interface (GUI) for pre- and post-processing of 2D and 3D SOFC-MP modelsCompleted reduced order modeling (ROM) tool
Compliant SealsEvaluated compliant seal performance and damage-healing evolution in multi-cell stack simulations under thermal cycling
Metallic InterconnectsDeveloped an experimental-modeling approach for prediction of interconnect lifetime using interfacial indentation tests of surface-modified, coated interconnects
3
SOFC-MP 3D Integration with FEM Software
Integration with ABAQUS and ANSYS FEM models implementedModels created in the FEM environment per guidelines and exportedMesh is read by SOFC-MP and the electrochemical model is solvedThermal distributions from the 3D simulation exportedStructural analysis run in the commercial FEM code using the exported temperature field data
August 19, 2014 4
FEMGeometry/Mesh
TemperatureField ThermalStressDistribution
3DSOFCMPAnalysis
FEAAnalysis
Example: SOFC-MP/ANSYS FEA Model
50-cell ANSYS co-flow stack w/ H2 fuel
August 19, 2014 5
FuelFuel
AirAir
SOFC-MP GUI
Graphical user interface replaces legacy MSC-MARC toolTabular menu structure provides pre-processing, job submission, job monitoring, and post-processing capabilities for both 2D and 3D SOFC-MP simulations
August 19, 2014 6
Fuel/AirFlowDirection
3DSOFCMPplanarcontoursforcells
SOFC-MP GUI (contd)
Cross-section plot of fuel temperature for 20-cell 2D model Effect of different fuel utilizations for cells #5 and #15 show higher peak temperature and gradient
August 19, 2014 7
Nominalflow Fuelmaldistribution
CellNum
ber
Bottomofstack
Topofstack
2DSOFCMPcrosssectioncontoursforstack
Fuel/AirFlowDirection
System Design Challenge
Ultimately, need design/engineering at several scales for successful SOFC commercializationModeling is practically limited by required computation times
Lower scales require smaller spatial resolutionHigher scales sacrifice detail or accuracy
Utilizing more details from the cell/stack level models to inform the system level model will allow more insight necessary for optimizing the BOP components and control strategies
August 19, 2014 8
ElectrodeMicrostructure IGFCPowerSystemMultiCellStackSingleCell
IncreasingScaleIncreasingScale
ResponseSurfaceAnalysis
ReducedOrderModel(ROM)
Reduced Order Model (ROM) Approach for SOFC Stacks
SamplingofNDimension
Space
CasestoRun
StackModel
StackResultsStackResultsStackResults
Regression
NInputVariablesand
Ranges
StackROM
MOutputVariables
NInputValues
MOutputValues
Slow
Fast
SOFC-ROM build
Aspen Plus use
MatricesforM
ResponseSurfaces
9August 19, 2014
SOFC-ROM: Visual Analysis Tools
Rich menu-driven plotting capabilities to aid understanding
visualize 2D-3D response surfacesplot sampling spaceactual vs. predicted values
output vs. input valuesoutput vs. output valuessensitivity chartserror histogramsresults as a function of S/C ratio
August 19, 2014 10
Example: Amount of On-Cell Reforming
Region with high current density and reduced temperature identified
August 19, 2014 11
Current
CH4
MaxTemp
H2CH4 H2
Example: Stack Peak Temperature Control
August 19, 2014 12
Evaluate stack maximum temperature as the stack size increasesE.g., identify required inlet temperature to ensure Tmax < 850C
Use exported ROMMaximum
Temperature
#CellsInletTemperature
Summary for SOFC-ROM
Implemented data validation toolsChecks predicted values from a created ROM against actual values to ensure ROM is suitable
Implemented scalable error estimation Previous 1-off estimation unsuitable for large number of sampled cases and replaced with 20/80 cross validation approach to test multiple parameter simultaneously
Implemented scalable visualizationPre-computation of data for rapid plotting replaced with dynamic generation for 2D or 3D graphs
Planned initial implementation is complete
Have initiated collaborative testing with BAH systems modelers to demonstrate utility for modeling of SOTA SOFC-based power systems
August 19, 2014 13
Seal Modeling Task Overview
Challenge:Seals must remain hermetic for stack operating lifetime
Goal: Develop quantitative models to capture the thermo-mechanical behaviors of the sealant glass materials and examine the durability ofthe compliant sealants under SOFC stack operation conditions
Technical Approach: Develop constitutive models to resolve the thermo-visco-elastic-damage-healing material behaviors of the sealant glassUse multi-scale modeling approaches to bridge the intrinsic material characteristics of the glass and its thermo-mechanical properties
Accomplishment: Completed model development and stack simulations to evaluate sealing performance under different operating conditions including thermal cycling
14
Modeling of the compliant SCN-1 glass
Constitutive thermo-visco-elastic-damage-healing model
15
Physically-driven damage and healing kinetics determined through lower-length scale simulations and experiments:
Pressure driven crack nucleationEnergy driven crack growthThermal diffusional crack healingHydrostatic-stress induced pore nucleationInelastic flow induced pore growth
damageisconsideredtobethefractionalreductioninelasticmodulus andformulatedas
Diffusionalhealing
Crackpropagation
XuW.,XSun,BJKoeppel,HZbib 2014.InternationalJournalofPlasticitydoi:10.1016/j.ijplas.2014.06.011
Finite Element Model of SOFC stack
16
FiniteelementanalysesperformedusingABAQUS
Compliantsealbondsthecelltothemetallicframe
Compliantglassmaterialmodelimplementedinthestacksimulationthroughsubroutines
PNNLs SECA Core Technology Program stack test fixture
Similar finite element models have also been created for larger planar designs that more closely resemble full-sized SECA cells and stacks.
Reliability of Multi-Cell SOFC Stack During Multiple Thermal Cycles
August 19, 2014 17
Mechanical integrity of the glass seal is minimally impacted by 10 deep and rapid thermal cycles
Stress and damage distributions within the three seals (from top to bottom) are almost the same; crack initiation is increased by accumulated pore-related damage which appears to saturate over time
Stress
Damage
Comparison of Mechanical Responses Between Sealant Glass Materials
18
max=1.9MPa max=21MPa
Compliant SCN-1 glass accumulates much less damage because of timely stress relaxation and its healing capability upon heating
Stress
DamageSCN1 G18:Astateoftheartdevitrifyingglass(Nguyenetal.,2006andStephensetal.,
2009)
August 19, 2014 19
Effects of Ceramic Fillers on Healing(Stack Simulation)
Healing time will increase with fiber volume fraction
exp
h1=4E-4 h2=0.2 h3=28.5
Note: here the existence of ceramic fillers is effectively considered through the activation energy of the healing probability function. In order to explicitly resolve the interaction between the reinforcement phase and the glass matrix as well as to establish a more generic description/prediction of the influence of the fillers, high resolution lower-length scale model is needed.
Required cooling/heating rates and durations during thermal cycling to sufficiently heal cracking damage can be determined
Summary for Seal Modeling
Simulation of the compliant seal material suggests that it a viable design option to consider for stack sealing
Cracking damage from thermal-cycling can be completely healedPore damage occurs but is small and can be mitigated with fillers
Description and capabilities of the model developed in this task are described in a recent summary report and journal article
YS Chou, JP Choi, W Xu, EV Stephens, BJ Koeppel, JW Stevenson, E Lara-Curzio (2014) Compliant Glass Seals for SOFC Stacks, PNNL-23397.W Xu, X Sun, E Stephens, I Mastorakos, MA Khaleel, HM Zbib (2012). A Mechanistic-Based Healing Model for Self-healing Glass Seals Used in Solid Oxide Fuel Cells, Journal of Power Sources 218:445-454.W Xu, X Sun, BJ Koeppel, HM Zbib (2014). A Continuum Thermo-Inelastic Model for Damage and Healing in Self-Healing Glass Materials, International Journal of Plasticity (in press).
August 19, 2014 20
Mechanical Reliability and Life Prediction of Coated Metallic Interconnects
Challenge:IC must meet SECA lifetime requirement
Goal: Use modeling to predict interconnect life under isothermal cooling and quantitatively estimate the effect of materials and geometry parameters on the interconnect life
Technical Approach: Develop a combined analytical/numerical approach based on the theory of bucking driven blistering to related the interface strength to the life prediction
Accomplishment: Evaluated the predicted statistical lifetime as a function of scatter in the strength measurements
21
Contributions to Long IC Lifetime
Different design features contribute jointly to mitigate degradation mechanisms and ensure long lifetime of the IC protection system
August 19, 2014 22
Coating
ScaleScale
Substrate
CoatingrestrictsO2 diffusiontoreducescalegrowthrate
Coatingstiffnessprovidesmechanicalsupport tohinderblisterbuckling
Substratesurfacemodificationsincreaseinterfacialstrength andcrackresistance topreventscalesubstratedelamination
Coatingcompatibilityprovidesverystrongcoatingscaleinterfacebond
Substratesurfacemodificationsincreasescaleadhesionpostdelaminationbymechanicalinterlocking
O2
CoatingCTEmatchedwithsubstratetominimizethermalstresses
FractureToughnessModel
CrossSectionSample
Preparation
InterfacialIndentationExperiments
IC Lifetime Analysis Methodology
August 19, 2014 23
CriticalLoadandCrackSize
MaterialProperties
OxideGrowthKineticsModel
Developed technical approach using experiments and modelingUncertainty analysis to capture scatter in the experimental data
LongTermHeatTreatmentExperiments
FractureToughness
CriticalOxideScaleThickness
OxideThickness
Measurements
DelaminationandBuckling
ModelICLifetime
ThermalLoading
Uncertainty
1) Indentation Experiments
Specimen Conditions
800-850C2k,10k, 14k, 20k, 26k, 30k hoursSurface blast (SB) and surface grind (SG)
Plot crack size versus load
August 19, 2014 24
2) Uncertainty in Critical Indentation Load
For the indent where a valid crack propagates along the interface, the log of the average crack size is plotted versus the log of the applied loadFor all indents with or without a crack, the log of the indent diagonal is plotted versus the log of the applied load (i.e., hardness)Linear regression is then used for each set of data
August 19, 2014 25
Intercept(mean)
Intercept(std dev)
Slope(mean)
Slope(stddev)
NoCrack 2.302 0.049 0.5 0
W/Crack 2.975 0.250 0.877 0.3901.8544
3) Uncertainty in KI
Using the mean and standard deviation statistics from the linear fits, determine the distribution for the interface toughness Perform 1000 Monte Carlo simulationsDetermine the probability distribution function (PDF) of ln(Pc), ln(ac), and KI
August 19, 2014 26
ln(Pc) ln(ac) KImean 1.78 1.41 2.99
stddev 0.68 0.35 0.51
-6 -4 -2 0 2 4 60
0.005
0.01
0.015
0.02
0.025
0.03
0.035
KIln(pc)
ln(ac)
27
Assume linear elastic materials with constant thermal expansion for three layersNext, evaluate the critical thickness hc and its uncertainty with derived distribution information on KI.
4) Uncertainty in hc
MechanicalPropertiesE,,
Thicknessesh
InterfaceToughness
KITemperature
ChangeT
hc(m)
mean 12.76
Stddev 2.51
5) IC Life from Oxidation Kinetic Curves
From hc, IC life can be identified from the oxidation kinetic curves.Long term oxidation found to better correlate with linear fit than parabolic fit
By this way, IC life can be quantitatively predicted, and the effect of interface toughness, coating property, etc. can be systematically investigated.
August 19, 2014 28
ScaleGrowthHistoryat800C ScaleGrowthHistoryat850C
Probability Density and Cumulative Distributions of Material Lifetime
Using the experimentally determined oxide growth rate and the KICdistribution, the predicted probability density function for the expected lifetime is obtainedThis is integrated to determine the cumulative distribution function
August 19, 2014 29
Lifetime(Hrs)
mean 55454
std dev 14499
ProbabilityDensityFunction CumulativeDistributionFunction
No Spalling
20kHr 99.9%
30kHr 99.0%
40kHr 84.0%
Initial Lifetime Estimates
Data scatterStill evaluating whether this is due to the methodology or the intrinsic variability of the specimens themselvesSB is generally better than SG, but SG has much wider range of estimated strength
Observations of cross-sections suggest that the grinding is non-uniform
Assuming the coupon results are representative of the entire IC, mean lifetimes of 34-57k hr at 800C for SB specimens
August 19, 2014 30
0 5000 10000 15000 20000 25000 3000020000
30000
40000
50000
60000
70000
80000
90000
SB 800C SG 800C
IC li
fe (H
rs)
Scale growth time (Hrs)
Sensitivity of Critical Scale Thickness
Evaluated effect of various parameters on critical oxide thickness hcMild compressive stress on the interconnect increases the hc
Areas under stack preload will be more resistant to delaminationThe coating itself acts a mechanical support for the scale to resist buckling, so thicker coating is beneficial to resist this failure mode
August 19, 2014 31
EffectofCompressiveStress EffectofCoatingThickness
Summary for Interconnect Modeling
August 19, 2014 32
The uncertainty in the IC life prediction was quantitatively derived from the variability in the indentation experimentsThe sensitivity of the critical oxide thickness to various other design parameters were evaluatedTrends in the IC lifetime evaluations are still being investigated, but the SB surface modification is more uniform than SG which showed wide variability in strength
Ongoing/Proposed Modeling Activities
Complete IC analysisContinue work with BAH/NETL modelers to implement and test a reduced order model made by the SOFC-ROM tool in IGFC/NGFC Aspen system modelsPerform mechanical reliability study of realistic state-of-art planar stack components and interfaces for different operating conditions and amount of on-cell reforming using SOFC-MP and FEM toolsSimulate new contact material fabrication methods and engineered surface textures to improve contact layer bulk and interfacial strengthEvaluate effects of residual stresses from contact layer fabrication on overall stack mechanical reliability
33
Acknowledgements
The work summarized in this presentation was funded by the U.S. Department of Energys Solid-State Energy Conversion Alliance (SECA) Core Technology Program
The authors wish to thank Shailesh Vora, Heather Quedenfeld, Briggs White, Rin Burke, Joe Stoffa, and Travis Shultz for their valuable guidance and technical discussions.
August 19, 2014 34